Plastics are a wide range of synthetic or semi-synthetic materials that use polymers as a main ingredient. Plastics are also considered organic materials, like wood, paper, or wool. Their plasticity makes it possible for plastics to be moulded, extruded or pressed into solid objects of various shapes. This adaptability, plus a wide range of other properties, such as being lightweight, durable, flexible, and inexpensive to produce, has led to its widespread use. Plastics typically are made through human industrial systems. Most modern plastics are derived from fossil fuel-based chemicals like natural gas or petroleum; however, recent industrial methods use variants made from renewable materials, such as corn or cotton derivatives.
In developed economies, about a third of plastic is used in packaging and roughly the same in buildings in applications such as piping, plumbing or vinyl siding. Other uses include automobiles (up to 20% plastic ), furniture, and toys. In the developing world, the applications of plastic may differ; 42% of India's consumption is used in packaging. In the medical field, polymer implants and other medical devices are derived at least partially from plastic. Worldwide, about 50 kg of plastic is produced annually per person, with production doubling every ten years.
The world's first fully synthetic plastic was Bakelite, invented in New York in 1907, by Leo Baekeland, who coined the term "plastics". Dozens of different types of plastics are produced today, such as polyethylene, which is widely used in product packaging, and polyvinyl chloride, used in construction and pipes because of its strength and durability. Many chemists have contributed to the materials science of plastics, including Nobel laureate Hermann Staudinger, who has been called "the father of polymer chemistry" and Herman Mark, known as "the father of polymer physics".
The success and dominance of plastics starting in the early 20th century has caused widespread environmental problems, due to their slow decomposition rate in natural ecosystems. Toward the end of the 20th century, the plastics industry promoted recycling in order to ease environmental concerns while continuing to produce virgin plastic. The main companies producing plastics doubted the economic viability of recycling at the time, and this is reflected in contemporary plastic collection. Plastic collection and recycling is largely ineffective because of failures of contemporary decision-making mechanisms that resulted in a complexity and amount of cleaning and sorting post-consumer plastics too high for contemporary methods. Most plastic produced has not been reused, either being captured in landfills or persisting in the environment as plastic pollution. Plastic pollution can be found in all the world's major water bodies, for example, creating garbage patches in all of the world's oceans and contaminating terrestrial ecosystems.
The word plastic derives from the Greek πλαστικός (plastikos) meaning "capable of being shaped or molded," and in turn from πλαστός (plastos) meaning "molded." As a noun the word most commonly refers to the solid products of petrochemical-derived manufacturing.
The noun plasticity refers specifically here to the deformability of the materials used in the manufacture of plastics. Plasticity allows molding, extrusion or compression into a variety of shapes: films, fibers, plates, tubes, bottles and boxes, among many others. Plasticity also has a technical definition in materials science outside the scope of this article referring to the non-reversible change in form of solid substances.
Most plastics contain organic polymers. The vast majority of these polymers are formed from chains of carbon atoms, with or without the attachment of oxygen, nitrogen or sulfur atoms. These chains comprise many repeating units formed from monomers. Each polymer chain consists of several thousand repeating units. The backbone is the part of the chain that is on the main path, linking together a large number of repeat units. To customize the properties of a plastic, different molecular groups called side chains hang from this backbone; they are usually hung from the monomers before the monomers themselves are linked together to form the polymer chain. The structure of these side chains influences the properties of the polymer.
Properties and classifications
Plastics are usually classified by the chemical structure of the polymer's backbone and side chains. Important groups classified in this way include the acrylics, polyesters, silicones, polyurethanes, and halogenated plastics. Plastics can be classified by the chemical process used in their synthesis, such as condensation, polyaddition, and cross-linking. They can also be classified by their physical properties, including hardness, density, tensile strength, thermal resistance, and glass transition temperature. Plastics can additionally be classified by their resistance and reactions to various substances and processes, such as exposure to organic solvents, oxidation, and ionizing radiation. Other classifications of plastics are based on qualities relevant to manufacturing or product design for a particular purpose. Examples include thermoplastics, thermosets, conductive polymers, biodegradable plastics, engineering plastics and elastomers.
Thermoplastics and thermosetting polymers
One important classification of plastics is the degree to which the chemical processes used to make them are reversible or not.
Thermoplastics do not undergo chemical change in their composition when heated and thus can be molded repeatedly. Examples include polyethylene (PE), polypropylene (PP), polystyrene (PS), and polyvinyl chloride (PVC).
Thermosets, or thermosetting polymers, can melt and take shape only once: after they have solidified, they stay solid. If reheated, thermosets decompose rather than melt. In the thermosetting process, an irreversible chemical reaction occurs. The vulcanization of rubber is an example of this process. Before heating in the presence of sulfur, natural rubber (polyisoprene) is a sticky, slightly runny material; after vulcanization, the product is dry and rigid.
Amorphous plastics and crystalline plastics
Many plastics are completely amorphous (without a highly ordered molecular structure), including thermosets, polystyrene, and methyl methacrylate (PMMA). Crystalline plastics exhibit a pattern of more regularly spaced atoms, such as high-density polyethylene (HDPE), polybutylene terephthalate (PBT), and polyether ether ketone (PEEK). However, some plastics are partially amorphous and partially crystalline in molecular structure, giving them both a melting point and one or more glass transitions (the temperature above which the extent of localized molecular flexibility is substantially increased). These so-called semi-crystalline plastics include polyethylene, polypropylene, polyvinyl chloride, polyamides (nylons), polyesters and some polyurethanes.
Intrinsically Conducting Polymers (ICP) are organic polymers that conduct electricity. While a conductivity of up to 80 kS/cm in stretch-oriented polyacetylene, has been achieved, it does not approach that of most metals. For example, copper has a conductivity of several hundred kS/cm.
Biodegradable plastics and bioplastics
Biodegradable plastics are plastics that degrade (break down) upon exposure to sunlight or ultra-violet radiation; water or dampness; bacteria; enzymes; or wind abrasion. Attack by insects, such as waxworms and mealworms, can also be considered as forms of biodegradation. Aerobic degradation requires that the plastic be exposed at the surface, whereas anaerobic degradation would be effective in landfill or composting systems. Some companies produce biodegradable additives to enhance biodegradation. Although starch powder can be added as a filler to allow some plastics to degrade more easily, such treatment does not lead to complete breakdown. Some researchers have genetically engineered bacteria to synthesize completely biodegradable plastics, such as polyhydroxybutyrate (PHB); however, these are relatively costly as of 2021.
While most plastics are produced from petrochemicals, bioplastics are made substantially from renewable plant materials like cellulose and starch. Due both to the finite limits of fossil fuel reserves and to rising levels of greenhouse gases caused primarily by the burning of those fuels, the development of bioplastics is a growing field.  Global production capacity for bio-based plastics is estimated at 327,000 tonnes per year. In contrast, global production of polyethylene (PE) and polypropylene (PP), the world's leading petrochemical-derived polyolefins, was estimated at over 150 million tonnes in 2015.
- Polyamides (PA) or (nylons): fibers, toothbrush bristles, tubing, fishing line, and low-strength machine parts, such as engine parts or gun frames
- Polycarbonate (PC): compact discs, eyeglasses, riot shields, security windows, traffic lights, and lenses
- Polyester (PES): fibers and textiles
- Polyethylene (PE): a wide range of inexpensive uses including supermarket bags and plastic bottles
- High-density polyethylene (HDPE): detergent bottles, milk jugs, and molded plastic cases
- Low-density polyethylene (LDPE): outdoor furniture, siding, floor tiles, shower curtains, and clamshell packaging
- Polyethylene terephthalate (PET): carbonated drink bottles, peanut butter jars, plastic film, and microwavable packaging
- Polypropylene (PP): bottle caps, drinking straws, yogurt containers, appliances, car fenders and bumpers, and plastic pressure pipe systems
- Polystyrene (PS): foam peanuts, food containers, plastic tableware, disposable cups, plates, cutlery, compact disc (CD) and cassette boxes
- High impact polystyrene (HIPS): refrigerator liners, food packaging and vending cups
- Polyurethanes (PU): cushioning foams, thermal insulation foams, surface coatings and printing rollers: currently the sixth or seventh most commonly-used plastic and, for instance, the most commonly used plastic in cars
- Polyvinyl chloride (PVC): plumbing pipes and guttering, electrical wire/cable insulation, shower curtains, window frames and flooring
- Polyvinylidene chloride (PVDC): food packaging, such as Saran
- Acrylonitrile butadiene styrene (ABS): electronic equipment cases (e.g. computer monitors, printers, keyboards) and drainage pipe
- Polycarbonate + acrylonitrile butadiene styrene (PC + ABS): a blend of PC and ABS that creates a stronger plastic used in car interior and exterior parts, and in mobile phone bodies
- Polyethylene + acrylonitrile butadiene styrene (PE + ABS): a slippery blend of PE and ABS used in low-duty dry bearings
- Furan: resin based on furfuryl alcohol used in foundry sands and biologically derived composites
- Maleimide/bismaleimide: used in high-temperature composite materials
- Melamine formaldehyde (MF): one of the aminoplasts, used as a multi-colorable alternative to phenolics, for instance in moldings (e.g., break-resistant alternatives to ceramic cups, plates and bowls for children) and the decorated top surface layer of the paper laminates (e.g., Formica)
- Phenolics or phenol formaldehyde (PF): high-modulus, relatively heat-resistant polymer with excellent fire resistance. Used for insulating parts in electrical fixtures, paper laminated products (e.g., Formica) and thermal-insulation foams. It is a thermosetting plastic, with the familiar trade name Bakelite, that can be molded by heat and pressure when mixed with a filler like wood flour, cast in its unfilled liquid form, or cast as foam (Oasis).
- Plastarch: biodegradable and heat-resistant thermoplastic composed of modified corn starch
- Polydiketoenamine (PDK): a new type of plastic that can be dipped in acid and reshaped endlessly (currently being lab tested)[timeframe?]
- Polyepoxide (epoxy): used as an adhesive, a potting agent for electrical components, and a matrix for composite materials with hardeners including amine, amide, and boron trifluoride
- Polyetheretherketone (PEEK): strong, chemical- and heat-resistant thermoplastic; its biocompatibility allows for use in medical implant applications and aerospace moldings. It is one of the most expensive commercial polymers.
- Polyetherimide (PEI) (Ultem): a high-temperature, chemically stable polymer that does not crystallize
- Polyimide: a high-temperature plastic used in materials such as Kapton tape
- Polylactic acid (PLA): a biodegradable thermoplastic converted into a variety of aliphatic polyesters derived from lactic acid, which in turn can be made by fermenting various agricultural products such as cornstarch, once made from dairy products
- Polymethyl methacrylate (PMMA) (acrylic): contact lenses (of the original "hard" variety), glazing (best known in this form by its various trade names around the world; e.g. Perspex, Plexiglas, and Oroglas), fluorescent-light diffusers, and rear light covers for vehicles. It also forms the basis of artistic and commercial acrylic paints, when suspended in water with the use of other agents.
- Polysulfone: high-temperature melt-processable resin used in membranes, filtration media, water heater dip tubes and other high-temperature applications
- Polytetrafluoroethylene (PTFE), or Teflon: heat-resistant, low-friction coatings used in non-stick surfaces for frying pans, plumber's tape and water slides
- Silicones (polysiloxanes): heat-resistant resins used mainly as sealants but also used for high-temperature cooking utensils and as a base resin for industrial paints
- Urea-formaldehyde (UF): one of the aminoplasts used as a multi-colorable alternative to phenolics: used as a wood adhesive (for plywood, chipboard, hardboard) and electrical switch housings
- Polyamide-imide (PAI): High-performance engineering plastic extensively used in high performance gears, switches, transmission and other automotive components, and aerospace parts.
The first plastic based on a synthetic polymer was invented in 1907, by Leo Hendrik Baekeland, a Belgian-born American living in New York State. He had been looking for an insulating shellac to coat wires in electric motors and generators. He discovered that combining phenol (C6H5OH) and formaldehyde (HCOH) formed a sticky mass and that the material could be mixed with wood flour, asbestos, or slate dust to create strong and fire-resistant "composite" materials. The new material tended to foam during synthesis, requiring that Baekeland build pressure vessels to force out the bubbles and provide a smooth, uniform product. Bakelite, named for himself and patented in 1909, was originally used for electrical and mechanical parts; it came into widespread use in general goods and jewelry in the 1920s. A purely synthetic material, Bakelite was also an early thermosetting plastic.
DuPont Corporation began a secret development project in 1927 designated Fiber66 under the direction of Harvard chemist Wallace Carothers and chemistry department director Elmer Keiser Bolton. Carothers's work led to the discovery of synthetic nylon fiber, which was very strong and flexible. The first application was for toothbrush bristles. Carothers and his team synthesized a number of different polyamides including polyamide 6.6 and 4.6, as well as polyesters.
Nylon was the first commercially successful synthetic thermoplastic polymer. The first women's nylon stockings (nylons) were introduced by DuPont at the 1939 World's Fair in New York City. It had taken 12 years and US$27 million to refine nylon and develop the industrial processes for its bulk manufacture. In 1940, 64 million pairs of nylons were sold.
When the US entered World War II, the capacity DuPont had developed to produce nylons shifted to manufacturing vast numbers of parachutes for fliers and paratroopers. After the war ended, DuPont resumed selling nylon to the public, engaging in a 1946 promotional campaign that brought on the so-called nylon riots.
Subsequently, polyamides 6, 10, 11, and 12 have been developed based on monomers that are ring compounds, such as caprolactam. Nylon 66 is a material manufactured by condensation polymerization. Nylon of different types remains an important plastic, and in its bulk form is very wear-resistant, particularly if oil-impregnated. It is used to build gears, plain bearings, valve seats, and seals; and because of good heat-resistance, increasingly for vehicular transportation applications, as well as for other mechanical parts.
Poly(methyl methacrylate) (PMMA), also known as acrylic or acrylic glass as well as by the trade names Plexiglas, Acrylite, Lucite, and Perspex, is a transparent thermoplastic often used in sheet form as a lightweight or shatter-resistant alternative to glass. PMMA can also be utilized as a casting resin, in inks and coatings, and has many other uses.
Unplasticised polystyrene is a rigid, brittle, inexpensive plastic that has been used to make plastic model kits and similar knick-knacks. It also is the basis for some of the most popular "foamed" plastics, under the name styrene foam or Styrofoam. Like most other foam plastics, foamed polystyrene can be manufactured in an "open cell" form, in which the foam bubbles are interconnected, as in an absorbent sponge, and "closed cell", in which all the bubbles are distinct, like tiny balloons, as in gas-filled foam insulation and flotation devices. In the late 1950s, high impact styrene was introduced, which was not brittle. It finds much current use as the substance of toy figurines and novelties.
Polyvinyl chloride (PVC, commonly called "vinyl")  incorporates chlorine atoms. C-Cl bonds in the backbone are hydrophobic and resist oxidation (and burning). PVC is stiff, strong, heat and weather resistant, properties that make it suitable for use in devices for plumbing, gutters, house siding, enclosures for computers and other electronics gear. PVC can also be softened with chemical processing, and in this form it is now used for shrink-wrap, food packaging, and rain gear.
All PVC polymers are degraded by heat and light. When this happens, hydrogen chloride is released into the atmosphere and oxidation of the compound occurs. Because hydrogen chloride readily combines with water vapor in the air to form hydrochloric acid, polyvinyl chloride is not recommended for long-term archival storage of silver, photographic film or paper (mylar is preferable).
Natural rubber is an elastomer (an elastic hydrocarbon polymer) that originally was derived from latex, a milky colloidal suspension found in specialised vessels in some plants. It is useful directly in this form (indeed, the first appearance of rubber in Europe was cloth waterproofed with unvulcanized latex from Brazil). However, in 1839, Charles Goodyear invented vulcanized rubber: a form of natural rubber heated with sulfur (and a few other chemicals), forming cross-links between polymer chains (vulcanization), improving elasticity and durability. In 1851, Nelson Goodyear added fillers to natural rubber materials to form ebonite.
The first fully synthetic rubber was synthesized by Sergei Lebedev in 1910. In World War II, supply blockades of natural rubber from South East Asia caused a boom in development of synthetic rubber, notably styrene-butadiene rubber. In 1941, annual production of synthetic rubber in the US was only 231 tonnes which increased to 840,000 tonnes in 1945. In the space race and nuclear arms race, Caltech researchers experimented with using synthetic rubbers for solid fuel for rockets. Ultimately, all large military rockets and missiles would use synthetic rubber based solid fuels, and they would also play a significant part in the civilian space effort.
Additives consists of various organic or inorganic compounds which are blended into plastics to enhance performance functionality. The amounts added can vary significantly; for instance as much as 70% of the weight of PVC can be plasticisers whereas pigments may account for less than 1%. Many controversies associated with plastics actually relate to the additives.[further explanation needed]
Typical additives include:
Plastic colorants are chemical compounds used to color plastic. Those compounds come in a form of dyes and pigments. The type of a colorant is chosen based on the type of a polymeric resin, that needs to be colored.  Dyes are usually used with polycarbonates, polystyrene and acrylic polymers. Pigments are better suited for use with polyolefins. 
The colorant must satisfy various constraints, for example, the compound must be chemically compatible with the base resin, be a suitable match with a color standard (see e.g. International Color Consortium), be chemically stable, which in this case means being able to survive the stresses and processing temperature (heat stability) in the fabrication process and be durable enough to match the life duration of the product.masterbatches (concentrates), a method which involves a concentrate being separated into resin, cube blends ("salt & pepper mixes" - dry blending) which are natural polymers, already sprayed into natural polymers, surface coating, and precolored resins, which involve using precolored materials to make manufacturing cheaper.
Fillers and Reinforcements
Despite appearing similar these additives serve different purposes. Fillers are inert low-cost materials added to the polymer to reduce cost and weight. Examples include chalk, starch, cellulose, wood flour, and zinc oxide. Reinforcements may be added to strengthen the polymer against mechanical damage. Examples include adding carbon fibre to form fibre-reinforced plastic.
Plasticizers are used to improve the flexibility and rheology of plastics and are important in making films and cable. By mass they are often the most abundant additives,  although this varies significantly between polymers. Around 80–90% of global production is used in PVC, which may itself consist of up to 70% plasticiser by mass. Cellulose plastics, such as cellophane, also use significant amounts of plasticizers. By comparison, little or no plasticizer is present in polyethylene terephthalate (PET). Phthalates remain the most common class of plasticisers, despite public concern over their potential health effects as endocrine disruptors.
Polymer stabilizers are important during the forming and casting of molten plastic but also prolong the life of the polymers by suppressing polymer degradation that results from UV-light, oxidation, and other forces. Typical stabilizers thus absorb UV light or function as antioxidants.
- Release agents
Release agents are used during the production of plastic items to prevent them sticking to the mold, for instance in injection moulding. Slip Additives are similarly used to prevent polyolefin films from adhering to metal surfaces during processing. Erucamide and oleamide are common examples.
Biocides are added to prevent the growth of organisms of the plastic surface. This is usually aimed at making the plastic antibacterial. The majority of biocides are added to soft PVC and foamed polyurethanes. Compounds include isothiazolinones, triclosan, arsenic and organotin compounds.
Pure plastics have low toxicity due to their insolubility in water, and because they have a large molecular weight, they are biochemically inert. Plastic products contain a variety of additives, however, some of which can be toxic. For example, plasticizers like adipates and phthalates are often added to brittle plastics like PVC to make them pliable enough for use in food packaging, toys, and many other items. Traces of these compounds can leach out of the product. Owing to concerns over the effects of such leachates, the EU has restricted the use of DEHP (di-2-ethylhexyl phthalate) and other phthalates in some applications, and the US has limited the use of DEHP, DPB, BBP, DINP, DIDP, and DnOP in children's toys and child-care articles through the Consumer Product Safety Improvement Act. Some compounds leaching from polystyrene food containers have been proposed to interfere with hormone functions and are suspected human carcinogens (cancer-causing substances). Other chemicals of potential concern include alkylphenols.
While a finished plastic may be non-toxic, the monomers used in the manufacture of its parent polymers may be toxic. In some cases, small amounts of those chemicals can remain trapped in the product unless suitable processing is employed. For example, the World Health Organization's International Agency for Research on Cancer (IARC) has recognized vinyl chloride, the precursor to PVC, as a human carcinogen.
Bisphenol A (BPA)
Some plastic products degrade to chemicals with estrogenic activity. The primary building block of polycarbonates, bisphenol A (BPA), is an estrogen-like endocrine disruptor that may leach into food. Research in Environmental Health Perspectives finds that BPA leached from the lining of tin cans, dental sealants and polycarbonate bottles can increase the body weight of lab animals' offspring. A more recent animal study suggests that even low-level exposure to BPA results in insulin resistance, which can lead to inflammation and heart disease. As of January 2010, the Los Angeles Times reported that the US Food and Drug Administration (FDA) is spending $30 million to investigate indications of BPA's link to cancer. Bis(2-ethylhexyl) adipate, present in plastic wrap based on PVC, is also of concern, as are the volatile organic compounds present in new car smell. The EU has a permanent ban on the use of phthalates in toys. In 2009, the US government banned certain types of phthalates commonly used in plastic.
The development of plastics has evolved from the use of naturally plastic materials (e.g., gums and shellac) to the use of the chemical modification of those materials (e.g., natural rubber, cellulose, collagen, and milk proteins), and finally to completely synthetic plastics (e.g., bakelite, epoxy, and PVC). Early plastics were bio-derived materials such as egg and blood proteins, which are organic polymers. In around 1600 BC, Mesoamericans used natural rubber for balls, bands, and figurines. Treated cattle horns were used as windows for lanterns in the Middle Ages. Materials that mimicked the properties of horns were developed by treating milk proteins with lye. In the nineteenth century, as chemistry developed during the Industrial Revolution, many materials were reported. The development of plastics accelerated with Charles Goodyear's 1839 discovery of vulcanization to harden natural rubber.
Parkesine, invented by Alexander Parkes in 1855 and patented the following year, is considered the first man-made plastic. It was manufactured from cellulose (the major component of plant cell walls) treated with nitric acid as a solvent. The output of the process (commonly known as cellulose nitrate or pyroxilin) could be dissolved in alcohol and hardened into a transparent and elastic material that could be molded when heated. By incorporating pigments into the product, it could be made to resemble ivory. Parkesine was unveiled at the 1862 International Exhibition in London and garnered for Parkes the bronze medal.
In 1893, French chemist Auguste Trillat discovered the means to insolubilize casein (milk proteins) by immersion in formaldehyde, producing material marketed as galalith. In 1897, mass-printing press owner Wilhelm Krische of Hanover, Germany, was commissioned to develop an alternative to blackboards. The resultant horn-like plastic made from casein was developed in cooperation with the Austrian chemist (Friedrich) Adolph Spitteler (1846–1940). Although unsuitable for the intended purpose, other uses would be discovered.
The world's first fully synthetic plastic was Bakelite, invented in New York in 1907 by Leo Baekeland, who coined the term plastics. Many chemists have contributed to the materials science of plastics, including Nobel laureate Hermann Staudinger, who has been called "the father of polymer chemistry," and Herman Mark, known as "the father of polymer physics."
After World War I, improvements in chemistry led to an explosion of new forms of plastics, with mass production beginning in the 1940s and 1950s. Among the earliest examples in the wave of new polymers were polystyrene (first produced by BASF in the 1930s) and polyvinyl chloride (first created in 1872 but commercially produced in the late 1920s). In 1923, Durite Plastics, Inc., was the first manufacturer of phenol-furfural resins. In 1933, polyethylene was discovered by Imperial Chemical Industries (ICI) researchers Reginald Gibson and Eric Fawcett.
The discovery of polyethylene terephthalate is credited to employees of the Calico Printers' Association in the UK in 1941; it was licensed to DuPont for the US and ICI otherwise, and as one of the few plastics appropriate as a replacement for glass in many circumstances, resulting in widespread use for bottles in Europe. In 1954 polypropylene was discovered by Giulio Natta and began to be manufactured in 1957. Also in 1954 expanded polystyrene (used for building insulation, packaging, and cups) was invented by Dow Chemical.
Plastics manufacturing is a major part of the chemical industry, and some of the world's largest chemical companies have been involved since the earliest days, such as the industry leaders BASF and Dow Chemical.
In 2014, sales of the top 50 companies amounted to US $961.3 billion. The firms came from some 18 countries in total, with more than half of the companies on the list being headquartered in the US. Many of the top 50 plastics companies were concentrated in just three countries: the US with 12, Japan with 8, and Germany with 6. BASF was the world's largest chemical producer for the ninth year in a row. 
Many properties of plastics are determined by standards specified by the ISO, such as:
- ISO 306 – Thermoplastics
Many of the properties of plastics are determined by UL Standards, tests specified by Underwriters Laboratories (UL), such as:
Because the chemical structure of most plastics renders them durable, they are resistant to many natural degradation processes. Much of this material may persist for centuries or longer, given the demonstrated persistence of structurally similar natural materials such as amber.
There are differing estimates of how much plastic waste has been produced in the last century. By one estimate, one billion tons of plastic waste have been discarded since the 1950s. Others estimate a cumulative human production of 8.3 billion tons of plastic, of which 6.3 billion tons is waste, with only 9% getting recycled.
The Ocean Conservancy reported that China, Indonesia, Philippines, Thailand, and Vietnam dump more plastic into the sea than all other countries combined. The rivers Yangtze, Indus, Yellow, Hai, Nile, Ganges, Pearl, Amur, Niger, and Mekong "transport 88% to 95% of the global [plastics] load into the sea."[verify quote punctuation]
The presence of plastics, particularly microplastics, within the food chain is increasing. In the 1960s microplastics were observed in the guts of seabirds, and since then have been found in increasing concentrations.  The long-term effects of plastics in the food chain are poorly understood. In 2009 it was estimated that 10% of modern waste was plastic, although estimates vary according to region. Meanwhile, 50% to 80% of debris in marine areas is plastic.
Efforts to reduce environmental effects of plastics may include reduction of plastics production and use, waste- and recycling-policies, and the proactive development and deployment of alternatives to plastics such as for sustainable packaging.
Microplastics are fragments of any type of plastic less than 5 mm (0.20 in) in length, according to the U.S. National Oceanic and Atmospheric Administration (NOAA) and the European Chemicals Agency. They cause pollution by entering natural ecosystems from a variety of sources, including cosmetics, clothing, and industrial processes.
Two classifications of microplastics are currently recognized. Primary microplastics include any plastic fragments or particles that are already 5.0 mm in size or less before entering the environment. These include microfibers from clothing, microbeads, and plastic pellets (also known as nurdles). Secondary microplastics arise from the degradation (breakdown) of larger plastic products through natural weathering processes after entering the environment. Such sources of secondary microplastics include water and soda bottles, fishing nets, plastic bags, microwave containers and tea bags. Both types are recognized to persist in the environment at high levels, particularly in aquatic and marine ecosystems, where they cause water pollution. However, microplastics also accumulate in the air and terrestrial ecosystems. The term macroplastics is used to differentiate microplastics from larger plastic waste, such as plastic bottles.Because plastics degrade slowly (often over hundreds to thousands of years), microplastics have a high probability of ingestion, incorporation into, and accumulation in the bodies and tissues of many organisms. The toxic chemicals that come from both the ocean and runoff can also biomagnify up the food chain. In terrestrial ecosystems, microplastics have been demonstrated to reduce the viability of soil ecosystems and reduce weight of earthworms. The cycle and movement of microplastics in the environment are not fully known, but research is currently underway to investigate the phenomenon. Deep layer ocean sediment surveys in China (2020) show the presence of plastics in deposition layers far older than the invention of plastics, leading to suspected underestimation of microplastics in surface sample ocean surveys.
Decomposition of plastics
Plastics degrade by a variety of processes, the most significant of which is usually photo-oxidation. Their chemical structure determines their fate. Polymers' marine degradation takes much longer as a result of the saline environment and cooling effect of the sea, contributing to the persistence of plastic debris in certain environments. Recent studies have shown, however, that plastics in the ocean decompose faster than had been previously thought, due to exposure to the sun, rain, and other environmental conditions, resulting in the release of toxic chemicals such as bisphenol A. However, due to the increased volume of plastics in the ocean, decomposition has slowed down. The Marine Conservancy has predicted the decomposition rates of several plastic products: It is estimated that a foam plastic cup will take 50 years, a plastic beverage holder will take 400 years, a disposable diaper will take 450 years, and fishing line will take 600 years to degrade.
Microbial species capable of degrading plastics are known to science, some of which are potentially useful for disposal of certain classes of plastic waste.
- In 1975, a team of Japanese scientists studying ponds containing waste water from a nylon factory discovered a strain of Flavobacterium that digests certain byproducts of nylon 6 manufacture, such as the linear dimer of 6-aminohexanoate. Nylon 4 (polybutyrolactam) can be degraded by the ND-10 and ND-11 strands of Pseudomonas sp. found in sludge, resulting in GABA (γ-aminobutyric acid) as a byproduct.
- Several species of soil fungi can consume polyurethane, including two species of the Ecuadorian fungus Pestalotiopsis. They can consume polyurethane both aerobically and anaerobically (such as at the bottom of landfills).
- Methanogenic microbial consortia degrade styrene, using it as a carbon source. Pseudomonas putida can convert styrene oil into various biodegradable plastic|biodegradable polyhydroxyalkanoates.
- Microbial communities isolated from soil samples mixed with starch have been shown to be capable of degrading polypropylene.
- The fungus Aspergillus fumigatus effectively degrades plasticized PVC.: 45–46 Phanerochaete chrysosporium has been grown on PVC in a mineral salt agar.: 76 </ref> P. chrysosporium, Lentinus tigrinus, A. niger, and A. sydowii can also effectively degrade PVC.: 122
- Phenol-formaldehyde, commonly known as Bakelite, is degraded by the white rot fungus P. chrysosporium.
- Acinetobacter has been found to partially degrade low-molecular-weight polyethylene oligomers. When used in combination, Pseudomonas fluorescens and Sphingomonas can degrade over 40% of the weight of plastic bags in less than three months. The thermophilic bacterium Brevibacillus borstelensis (strain 707) was isolated from a soil sample and found capable of using low-density polyethylene as a sole carbon source when incubated at 50°C. Pre-exposure of the plastic to ultraviolet radiation broke chemical bonds and aided biodegradation; the longer the period of UV exposure, the greater the promotion of the degradation.
- Hazardous molds have been found aboard space stations that degrade rubber into a digestible form.
- Several species of yeasts, bacteria, algae and lichens have been found growing on synthetic polymer artifacts in museums and at archaeological sites.
- In the plastic-polluted waters of the Sargasso Sea, bacteria have been found that consume various types of plastic; however, it is unknown to what extent these bacteria effectively clean up poisons rather than simply release them into the marine microbial ecosystem.
- Plastic-eating microbes also have been found in landfills.
- Nocardia can degrade PET with an esterase enzyme.
- The fungus Geotrichum candidum, found in Belize, has been found to consume the polycarbonate plastic found in CDs.
- Futuro houses are made of fiberglass-reinforced polyesters, polyester-polyurethane, and PMMA. One such house was found to be harmfully degraded by Cyanobacteria and Archaea.
Plastic recycling encompasses a number of processes through which plastic waste is collected and converted back into useful products, instead of being simply disposed of. When performed correctly, plastic recycling can reduce dependence on landfill, conserve resources and protect the environment from plastic pollution and greenhouse gas emissions.
Increasing public awareness of plastic pollution has raised demand for plastic recycling, but it remains challenging from a technical and economic standpoint, causing it to lag behind the recycling rates of materials like aluminium, glass and paper. In general, there are many types of plastic and these need to be segregated from one another prior to recycling as they give a poor-quality product if mixed. Even when properly sorted and cleaned, the most common form of recycling in which plastic is re-melted and reformed into new items, usually results in polymer degradation at a chemical level, so that quality cannot be maintained. More advanced technologies which may mitigate this degradation suffer from high capital costs and are more energy hungry. Thus, even though recycling rates are improving, much of this activity merely delays rather than prevents the eventual disposal of plastic as waste. Regardless, life-cycle assessments show recycling in its various forms to be a net good for the environment.
Since the beginning of plastic production in the 20th century, until 2015, the world has produced some 6.3 billion tonnes of plastic waste, of which 9% has been recycled—only ~1% of total plastic has ever been recycled more than once. The global recycling rate in 2015 was 19.5%, while 25.5% was incinerated and the remaining 55% disposed of to landfill. Only ~2% was recycled in a sustainable closed-loop manner. As of 2019, due to limitations in economic viability, there is little incentive for companies to make a meaningful contribution to the plastic recycling supply chain. The plastics industry has known since the 1970s that recycling of most plastics is unlikely because of these economic limitations. However, the industry has continued to lobby for the expansion of recycling programs while at the same time increasing the amount of virgin plastic being produced.Almost all plastic is non-biodegradable and thus causes systematic harm to natural ecosystems. For example, approximately 8 million tons of waste plastic enter the Earth's oceans every year, causing damage to the aquatic ecosystem and large ocean garbage patches. Recycling and other forms of utilisation, such as energy recovery, can be part of reducing plastic in the waste stream, but does not alleviate the environmental unsustainability of the plastics industry.
According to one report, plastic contributed greenhouse gases in the equivalent of 850 million tons of carbon dioxide (CO2) to the atmosphere in 2019. Emissions could grow to 1.34 billion tons by 2030. By 2050, plastic could emit 56 billion tons of greenhouse gas emissions, as much as 14% of the earth's remaining carbon budget.
The effect of plastics on global warming is mixed. Plastics are generally made from petroleum, thus the production of plastics creates further emissions. However, due to the lightness and durability of plastic versus glass or metal, plastic may reduce energy consumption. For example, packaging beverages in PET plastic rather than glass or metal is estimated to save 52% in transportation energy.
Production of plastics
Production of plastics from crude oil requires 7.9 to 13.7 kWh/lb (taking into account the average efficiency of US utility stations of 35%). Producing silicon and semiconductors for modern electronic equipment is even more energy consuming: 29.2 to 29.8 kWh/lb for silicon, and about 381 kWh/lb for semiconductors. This is much higher than the energy needed to produce many other materials. For example, to produce iron (from iron ore) requires 2.5-3.2 kWh/lb of energy; glass (from sand, etc.) 2.3–4.4 kWh/lb; steel (from iron) 2.5–6.4 kWh/lb; and paper (from timber) 3.2–6.4 kWh/lb.
Incineration of plastics
Controlled high-temperature incineration, above 850°C for two seconds, performed with selective additional heating, breaks down toxic dioxins and furans from burning plastic, and is widely used in municipal solid waste incineration. Municipal solid waste incinerators also normally include flue gas treatments to reduce pollutants further. This is needed because uncontrolled incineration of plastic produces polychlorinated dibenzo-p-dioxins, a carcinogen (cancer causing chemical). The problem occurs because the heat content of the waste stream varies. Open-air burning of plastic occurs at lower temperatures, and normally releases such toxic fumes.
- Corn construction
- Light activated resin
- Molding (process)
- Organic light emitting diode
- Plastic film
- Plastic recycling
- Plastics engineering
- Plastics extrusion
- Biodegradable plastic
- Organisms breaking down plastic
- Progressive bag alliance
- Roll-to-roll processing
- Self-healing plastic
- Thermal cleaning
- Timeline of materials technology
- "What are plastics". www.plasticseurope.org. Retrieved 2021-09-17.
- "Life Cycle of a Plastic Product". Americanchemistry.com. Archived from the original on 2010-03-17. Retrieved 2011-07-01.
- Andrady AL, Neal MA (July 2009). "Applications and societal benefits of plastics". Philosophical Transactions of the Royal Society of London. Series B, Biological Sciences. 364 (1526): 1977–84. doi:10.1098/rstb.2008.0304. PMC 2873019. PMID 19528050.
- American Chemical Society National Historic Chemical Landmarks. "Bakelite: The World's First Synthetic Plastic". Retrieved 23 February 2015.
- Edgar D, Edgar R (2009). Fantastic Recycled Plastic: 30 Clever Creations to Spark Your Imagination. Sterling Publishing Company, Inc. ISBN 978-1-60059-342-0 – via Google Books.
- Teegarden DM (2004). Polymer Chemistry: Introduction to an Indispensable Science. NSTA Press. ISBN 978-0-87355-221-9 – via Google Books.
- "Plastikos" πλαστι^κ-ός. Henry George Liddell, Robert Scott, A Greek-English Lexicon. Retrieved 2011-07-01.
- "Plastic". Online Etymology Dictionary. Retrieved 2021-07-29.
- Ebbing D, Gammon SD (2016). General Chemistry. Cengage Learning. ISBN 978-1-305-88729-9.
- "Classification of Plastics". Joanne and Steffanie's Plastics Web Site. Archived from the original on 2007-12-15. Retrieved 2011-07-01.
- Kent R. "Periodic Table of Polymers". Plastics Consultancy Network. Archived from the original on 2008-07-03.
- "Composition and Types of Plastic". Infoplease.
- Gilleo K (2004). Area Array Packaging Processes: For BGA, Flip Chip, and CSP. McGraw Hill Professional. ISBN 978-0-07-142829-3 – via Google Books.
- Kutz M (2002). Handbook of Materials Selection. John Wiley & Sons. ISBN 978-0-471-35924-1 – via Google Books.
- Heeger AJ, Kivelson S, Schrieffer JR, Su WP (1988). "Solitons in Conducting Polymers". Reviews of Modern Physics. 60 (3): 781–850. Bibcode:1988RvMP...60..781H. doi:10.1103/RevModPhys.60.781.
- "Properties of Copper". Copper Development Association.
- Brandl H, Püchner P (1992). "Biodegradation Biodegradation of Plastic Bottles Made from 'Biopol' in an Aquatic Ecosystem Under In Situ Conditions". Biodegradation. 2 (4): 237–43. doi:10.1007/BF00114555. S2CID 37486324.
- "Archived copy". Archived from the original on 2011-07-20. Retrieved 2011-03-24.CS1 maint: archived copy as title (link)
- "Bioplastics industry shows dynamic growth". 5 December 2019.
- "Becoming Employed in a Growing Bioplastics Industry - bioplastics MAGAZINE". www.bioplasticsmagazine.com.
- Galie F (November 2016). "Global Market Trends and Investments in Polyethylene and Polyproplyene" (PDF). ICIS Whitepaper. Reed business Information, Inc. Retrieved 16 December 2017.
- "Scientists could have finally created the 'holy grail' of plastic". The Independent. 2019-05-09. Retrieved 2019-05-10.
- "Polymers in aerospace applications". Euroshore. Retrieved 2021-06-02.
- Watson, Peter. A Terrible Beauty (also published as Modern Mind: An intellectual history of the 20th century). London: Weidenfeld & Nicolson Ltd (imprint of Orion Books). 2001
- Kinnane A (2002). DuPont: From the banks of the Brandywine to miracles of science. Baltimore, MD: Johns Hopkins University Press. pp. 116–125. ISBN 978-0-8018-7059-0.
- Jezek G. "What is Vinyl?". Retrieved 9 January 2011.
- "Polyvinyl chloride". Plasticsusa.com. Archived from the original on 15 July 2011. Retrieved 9 January 2011.
- Salocks C, Kaley KB (2 February 2004). "Technical Support Document: Toxicology of Hydrogen Chloride (Revised)" (PDF). California EPA, Office of Environmental Health Hazard Assessment. p. 8. Archived from the original (PDF) on 4 November 2010. Retrieved 9 January 2011.
- "How can I preserve my family photographs for my grandchildren?". The Library of Congress Preservation FAQs. LoC. Retrieved 9 January 2011.
- Seymour RB, Deaning RD (1987). History of Polymeric Composites. VSP. p. 374.
- Hahladakis JN, Velis CA, Weber R, Iacovidou E, Purnell P (February 2018). "An overview of chemical additives present in plastics: Migration, release, fate and environmental impact during their use, disposal and recycling". Journal of Hazardous Materials. 344: 179–199. doi:10.1016/j.jhazmat.2017.10.014. PMID 29035713.
- Hans-Georg Elias "Plastics, General Survey" in Ullmann's Encyclopedia of Industrial Chemistry, 2005, Wiley-VCH, Weinheim. doi:10.1002/14356007.a20_543
- Teuten EL, Saquing JM, Knappe DR, Barlaz MA, Jonsson S, Björn A, et al. (July 2009). "Transport and release of chemicals from plastics to the environment and to wildlife". Philosophical Transactions of the Royal Society of London. Series B, Biological Sciences. 364 (1526): 2027–45. doi:10.1098/rstb.2008.0284. PMC 2873017. PMID 19528054.
- Nishikants (2013-06-28). "Plastic colorant and its role in plastic industry". Share and Discover Knowledge on LinkedIn SlideShare. Retrieved 2017-07-18.
- "Plastic Colorants Guide for Injection Molded Parts". RevPart. 2016-01-26. Retrieved 2017-07-18.
- Sepe M (2012-01-28). "Working with Color Concentrates". Plastics Technology. Retrieved 2017-07-18.
- "Colorants for Plastic Industry,Dyes for Plastics Industry,Pigments for Plastics Industry". Dyes and Pigments, Dyes Manufacturers, Dyes Intermediates, Pigments Suppliers, Wholesale Dyes Intermediates. Archived from the original on 2019-03-04. Retrieved 2017-07-18.
- "Toxics in Packaging Clearinghouse". Collation of Northeastern Governors (CONEG).
- "Methods of Coloring Plastics". RTP Company. Retrieved 2017-07-18.
- "Effect of coloring methods on properties of plastics". Polyplastics.com. Retrieved 2017-07-18.
- Kulshreshtha AK, Vasile C (2002). Handbook of Polymer Blends and Composites. iSmithers Rapra Publishing. ISBN 978-1-85957-249-8.
- U.S. Environmental Protection Agency (2005). Environmental Profiles of Chemical Flame-Retardant Alternatives for Low-Density Polyurethane Foam (Report). EPA 742-R-05-002A. Retrieved 4 April 2013.
- David F. Cadogan and Christopher J. Howick "Plasticizers" in Ullmann's Encyclopedia of Industrial Chemistry 2000, Wiley-VCH, Weinheim. doi:10.1002/14356007.a20_439
- Hahladakis JN, Velis CA, Weber R, Iacovidou E, Purnell P (February 2018). "An overview of chemical additives present in plastics: Migration, release, fate and environmental impact during their use, disposal and recycling". Journal of Hazardous Materials. 344: 179–199. doi:10.1016/j.jhazmat.2017.10.014. PMID 29035713.
- McRandle PW (March–April 2004). "Plastic Water Bottles". National Geographic. Retrieved 2007-11-13.
- Yang CZ, Yaniger SI, Jordan VC, Klein DJ, Bittner GD (July 2011). "Most plastic products release estrogenic chemicals: a potential health problem that can be solved". Environmental Health Perspectives. 119 (7): 989–96. doi:10.1289/ehp.1003220. PMC 3222987. PMID 21367689.
- Rubin BS, Murray MK, Damassa DA, King JC, Soto AM (July 2001). "Perinatal exposure to low doses of bisphenol A affects body weight, patterns of estrous cyclicity, and plasma LH levels". Environmental Health Perspectives. 109 (7): 675–80. doi:10.2307/3454783. JSTOR 3454783. PMC 1240370. PMID 11485865.
- Alonso-Magdalena P, Morimoto S, Ripoll C, Fuentes E, Nadal A (January 2006). "The estrogenic effect of bisphenol A disrupts pancreatic beta-cell function in vivo and induces insulin resistance". Environmental Health Perspectives. 114 (1): 106–12. doi:10.1289/ehp.8451. PMC 1332664. PMID 16393666. Archived from the original on 2009-01-19.
- Zajac A (2010-01-16). "FDA Issues BPA Guidelines". Los Angeles Times. Retrieved 2021-07-29.
- McCormick LW (30 October 2009). "More Kids' Products Found Containing Unsafe Chemicals". ConsumerAffairs.com.
- UK Patent office (1857). Patents for inventions. UK Patent office. p. 255.
- "Dictionary – Definition of celluloid". Websters-online-dictionary.org. Archived from the original on 2009-12-11. Retrieved 2011-10-26.
- Fenichell S (1996). Plastic : the making of a synthetic century. New York: HarperBusiness. p. 17. ISBN 978-0-88730-732-4.
- Trimborn C (August 2004). "Jewelry Stone Make of Milk". GZ Art+Design. Retrieved 2010-05-17.
- Thompson RC, Swan SH, Moore CJ, vom Saal FS (July 2009). "Our plastic age". Philosophical Transactions of the Royal Society of London. Series B, Biological Sciences. 364 (1526): 1973–6. doi:10.1098/rstb.2009.0054. PMC 2874019. PMID 19528049.
- "Historical Overview and Industrial Development". International Furan Chemicals, Inc. Retrieved 4 May 2014.
- Tullo AH (27 July 2015). "Global Top 50 Chemical Companies". Chemical & Engineering News. American Chemical Society. Retrieved 27 October 2015.
- Weisman A (2007). The world without us. New York: Thomas Dunne Books/St. Martin's Press. ISBN 978-1-4434-0008-4.
- Geyer R, Jambeck JR, Law KL (July 2017). "Production, use, and fate of all plastics ever made". Science Advances. 3 (7): e1700782. Bibcode:2017SciA....3E0782G. doi:10.1126/sciadv.1700782. PMC 5517107. PMID 28776036.
- Leung H (21 April 2018). "Five Asian Countries Dump More Plastic Into Oceans Than Anyone Else Combined: How You Can Help". Forbes. Retrieved 23 June 2019.
China, Indonesia, Philippines, Thailand, and Vietnam are dumping more plastic into oceans than the rest of the world combined, according to a 2017 report by Ocean Conservancy
- Schmidt C, Krauth T, Wagner S (November 2017). "Export of Plastic Debris by Rivers into the Sea" (PDF). Environmental Science & Technology. 51 (21): 12246–12253. Bibcode:2017EnST...5112246S. doi:10.1021/acs.est.7b02368. PMID 29019247.
The 10 top-ranked rivers transport 88–95% of the global load into the sea
- Franzen H (30 November 2017). "Almost all plastic in the ocean comes from just 10 rivers". Deutsche Welle. Retrieved 18 December 2018.
It turns out that about 90 percent of all the plastic that reaches the world's oceans gets flushed through just 10 rivers: The Yangtze, the Indus, Yellow River, Hai River, the Nile, the Ganges, Pearl River, Amur River, the Niger, and the Mekong (in that order).
- Barnes DK, Galgani F, Thompson RC, Barlaz M (July 2009). "Accumulation and fragmentation of plastic debris in global environments". Philosophical Transactions of the Royal Society of London. Series B, Biological Sciences. 364 (1526): 1985–98. doi:10.1098/rstb.2008.0205. PMC 2873009. PMID 19528051.
- Blair Crawford, Christopher; Quinn, Brian (2016). Microplastic Pollutants (1st ed.). Elsevier Science. ISBN 9780128094068.[page needed]
- Arthur, Courtney; Baker, Joel; Bamford, Holly (2009). "Proceedings of the International Research Workshop on the Occurrence, Effects and Fate of Microplastic Marine Debris" (PDF). NOAA Technical Memorandum.
- Collignon, Amandine; Hecq, Jean-Henri; Galgani, François; Collard, France; Goffart, Anne (2014). "Annual variation in neustonic micro- and meso-plastic particles and zooplankton in the Bay of Calvi (Mediterranean–Corsica)" (PDF). Marine Pollution Bulletin. 79 (1–2): 293–8. doi:10.1016/j.marpolbul.2013.11.023. PMID 24360334.
- European Chemicals Agency. "Restricting the use of intentionally added microplastic particles to consumer or professional use products of any kind". ECHA. European Commission. Retrieved 8 September 2020.
- Cole, Matthew; Lindeque, Pennie; Fileman, Elaine; Halsband, Claudia; Goodhead, Rhys; Moger, Julian; Galloway, Tamara S. (2013). "Microplastic Ingestion by Zooplankton" (PDF). Environmental Science & Technology. 47 (12): 6646–55. Bibcode:2013EnST...47.6646C. doi:10.1021/es400663f. hdl:10871/19651. PMID 23692270.
- "Where Does Marine Litter Come From?". Marine Litter Facts. British Plastics Federation. Retrieved 2018-09-25.
- Boucher, Julien; Friot, Damien (2017). Primary microplastics in the oceans: A global evaluation of sources. doi:10.2305/IUCN.CH.2017.01.en. ISBN 978-2-8317-1827-9.
- Conkle, Jeremy L.; Báez Del Valle, Christian D.; Turner, Jeffrey W. (2018). "Are We Underestimating Microplastic Contamination in Aquatic Environments?". Environmental Management. 61 (1): 1–8. Bibcode:2018EnMan..61....1C. doi:10.1007/s00267-017-0947-8. PMID 29043380. S2CID 40970384.
- "Plastic free July: How to stop accidentally consuming plastic particles from packaging". Stuff. 2019-07-11. Retrieved 2021-04-13.
- "Development solutions: Building a better ocean". European Investment Bank. Retrieved 2020-08-19.
- Chamas, Ali; Moon, Hyunjin; Zheng, Jiajia; Qiu, Yang; Tabassum, Tarnuma; Jang, Jun Hee; Abu-Omar, Mahdi; Scott, Susannah L.; Suh, Sangwon (2020). "Degradation Rates of Plastics in the Environment". ACS Sustainable Chemistry & Engineering. 8 (9): 3494–3511. doi:10.1021/acssuschemeng.9b06635.
- Klein S, Dimzon IK, Eubeler J, Knepper TP (2018). "Analysis, Occurrence, and Degradation of Microplastics in the Aqueous Environment.". In Wagner M, Lambert S (eds.). Freshwater Microplastics. The Handbook of Environmental Chemistry. 58. Cham.: Springer. pp. 51–67. doi:10.1007/978-3-319-61615-5_3. ISBN 978-3-319-61614-8. See Section 3, "Environmental Degradation of Synthetic Polymers".
- Grossman, Elizabeth (2015-01-15). "How Plastics from Your Clothes Can End up in Your Fish". Time.
- "How Long Does it Take Trash to Decompose". 4Ocean. 20 January 2017. Archived from the original on 25 September 2018. Retrieved 25 September 2018.
- "Why food's plastic problem is bigger than we realise". www.bbc.com. Retrieved 2021-03-27.
- Nex, Sally (2021). How to garden the low carbon way: the steps you can take to help combat climate change (First American ed.). New York. ISBN 978-0-7440-2928-4. OCLC 1241100709.
- Xue B, Zhang L, Li R, Wang Y, Guo J, Yu K, Wang S (February 2020). "Underestimated Microplastic Pollution Derived from Fishery Activities and "Hidden" in Deep Sediment". Environmental Science & Technology. 54 (4): 2210–2217. doi:10.1021/acs.est.9b04850. PMID 31994391. Lay summary – ECO Magazine.
- American Chemical Society. "Plastics In Oceans Decompose, Release Hazardous Chemicals, Surprising New Study Says". Science Daily. Science Daily. Retrieved 15 March 2015.
- Le Guern C (March 2018). "When The Mermaids Cry: The Great Plastic Tide". Coastal Care. Archived from the original on 5 April 2018. Retrieved 10 November 2018.
- Kinoshita S, Kageyama S, Iba K, Yamada Y, Okada H (1975). "Utilization of a Cyclic Dimer and Linear Oligomers of E-Aminocaproic Acid by Achromobacter Guttatus". Agricultural and Biological Chemistry. 39 (6): 1219–1223. doi:10.1271/bbb1961.39.1219.
- Tokiwa Y, Calabia BP, Ugwu CU, Aiba S (August 2009). "Biodegradability of plastics". International Journal of Molecular Sciences. 10 (9): 3722–42. doi:10.3390/ijms10093722. PMC 2769161. PMID 19865515.
- Russell JR, Huang J, Anand P, Kucera K, Sandoval AG, Dantzler KW, et al. (September 2011). "Biodegradation of polyester polyurethane by endophytic fungi". Applied and Environmental Microbiology. 77 (17): 6076–84. Bibcode:2011ApEnM..77.6076R. doi:10.1128/aem.00521-11. PMC 3165411. PMID 21764951.
- Russell JR, Huang J, Anand P, Kucera K, Sandoval AG, Dantzler KW, et al. (September 2011). "Biodegradation of polyester polyurethane by endophytic fungi". Applied and Environmental Microbiology. 77 (17): 6076–84. Bibcode:2011ApEnM..77.6076R. doi:10.1128/AEM.00521-11. PMC 3165411. PMID 21764951.
- "Deep Geologic Repository Project" (PDF). Ceaa-acee.gc.ca. Retrieved 2017-04-18.
- Roy R (2006-03-07). "Immortal Polystyrene Foam Meets its Enemy". Livescience.com. Retrieved 2017-04-18.
- Ward PG, Goff M, Donner M, Kaminsky W, O'Connor KE (April 2006). "A two step chemo-biotechnological conversion of polystyrene to a biodegradable thermoplastic". Environmental Science & Technology. 40 (7): 2433–7. Bibcode:2006EnST...40.2433W. doi:10.1021/es0517668. PMID 16649270.
- Cacciari I, Quatrini P, Zirletta G, Mincione E, Vinciguerra V, Lupattelli P, Giovannozzi Sermanni G (November 1993). "Isotactic polypropylene biodegradation by a microbial community: physicochemical characterization of metabolites produced". Applied and Environmental Microbiology. 59 (11): 3695–700. Bibcode:1993ApEnM..59.3695C. doi:10.1128/AEM.59.11.3695-3700.1993. PMC 182519. PMID 8285678.
- Ishtiaq AM (2011). Microbial Degradation of Polyvinyl Chloride Plastics (PDF) (Ph.D.). Islamabad: Quaid-i-Azam University.
- Gusse AC, Miller PD, Volk TJ (July 2006). "White-rot fungi demonstrate first biodegradation of phenolic resin". Environmental Science & Technology. 40 (13): 4196–9. Bibcode:2006EnST...40.4196G. doi:10.1021/es060408h. PMID 16856735.
- "CanadaWorld – WCI student isolates microbe that lunches on plastic bags". The Record.com. Archived from the original on 2011-07-18.
- Hadad D, Geresh S, Sivan A (2005). "Biodegradation of polyethylene by the thermophilic bacterium Brevibacillus borstelensis". Journal of Applied Microbiology. 98 (5): 1093–100. doi:10.1111/j.1365-2672.2005.02553.x. PMID 15836478. S2CID 2977246.
- Bell TE (2007). "Preventing "Sick" Spaceships".
- Cappitelli F, Sorlini C (February 2008). "Microorganisms attack synthetic polymers in items representing our cultural heritage". Applied and Environmental Microbiology. 74 (3): 564–9. Bibcode:2008ApEnM..74..564C. doi:10.1128/AEM.01768-07. PMC 2227722. PMID 18065627.
- Zaikab GD (March 2011). "Marine Microbes Digest Plastic". Nature. doi:10.1038/news.2011.191.
- Bosch X (2001). "Fungus Eats CD". Nature. doi:10.1038/news010628-11.
- "Fungus 'Eats' CDs". BBC News. 22 June 2001.
- Cappitelli F, Principi P, Sorlini C (August 2006). "Biodeterioration of modern materials in contemporary collections: can biotechnology help?". Trends in Biotechnology. 24 (8): 350–4. doi:10.1016/j.tibtech.2006.06.001. PMID 16782219.
- Rinaldi A (November 2006). "Saving a fragile legacy. Biotechnology and microbiology are increasingly used to preserve and restore the world's cultural heritage". EMBO Reports. 7 (11): 1075–9. doi:10.1038/sj.embor.7400844. PMC 1679785. PMID 17077862.
- Hopewell, Jefferson; Dvorak, Robert; Kosior, Edward (27 July 2009). "Plastics recycling: challenges and opportunities". Philosophical Transactions of the Royal Society B: Biological Sciences. 364 (1526): 2115–2126. doi:10.1098/rstb.2008.0311. PMC 2873020. PMID 19528059.
- Al-Salem, S.M.; Lettieri, P.; Baeyens, J. (October 2009). "Recycling and recovery routes of plastic solid waste (PSW): A review". Waste Management. 29 (10): 2625–2643. doi:10.1016/j.wasman.2009.06.004. PMID 19577459.
- Ignatyev, I.A.; Thielemans, W.; Beke, B. Vander (2014). "Recycling of Polymers: A Review". ChemSusChem. 7 (6): 1579–1593. doi:10.1002/cssc.201300898. PMID 24811748.
- Geyer, Roland; Kuczenski, Brandon; Zink, Trevor; Henderson, Ashley (October 2016). "Common Misconceptions about Recycling". Journal of Industrial Ecology. 20 (5): 1010–1017. doi:10.1111/jiec.12355. S2CID 153936564.
- Lazarevic, David; Aoustin, Emmanuelle; Buclet, Nicolas; Brandt, Nils (December 2010). "Plastic waste management in the context of a European recycling society: Comparing results and uncertainties in a life cycle perspective". Resources, Conservation and Recycling. 55 (2): 246–259. doi:10.1016/j.resconrec.2010.09.014.
- Geyer, Roland; Jambeck, Jenna R.; Law, Kara Lavender (July 2017). "Production, use, and fate of all plastics ever made". Science Advances. 3 (7): e1700782. Bibcode:2017SciA....3E0782G. doi:10.1126/sciadv.1700782. PMC 5517107. PMID 28776036.
- "The New Plastics Economy: Rethinking the future of plastics & catalysing action". www.ellenmacarthurfoundation.org. Retrieved 28 May 2021.
- "Municipal sector grapples with plastic realities". Plastics Recycling Update. 5 September 2019. Retrieved 5 September 2019.
- National Public Radio, 12 September 2020 "How Big Oil Misled The Public Into Believing Plastic Would Be Recycled"
- PBS, Frontline, 31 March 2020, "Plastics Industry Insiders Reveal the Truth About Recycling"
- Hardesty, Britta Denise; Chris Wilcox (13 February 2015). "8 million tons of plastic are going into the ocean each year". The Conversation. Retrieved 21 February 2015.
- Jambeck, Jenna, Science 13 February 2015: Vol. 347 no. 6223; et al. (2015). "Plastic waste inputs from land into the ocean". Science. 347 (6223): 768–771. Bibcode:2015Sci...347..768J. doi:10.1126/science.1260352. PMID 25678662. S2CID 206562155.
- "Sweeping New Report on Global Environmental Impact of Plastics Reveals Severe Damage to Climate". Center for International Environmental Law (CIEL). 15 May 2019. Retrieved 16 May 2019.
- De Decker K (June 2009). Grosjean V (ed.). "The monster footprint of digital technology". Low-Tech Magazine. Retrieved 2017-04-18.
- "How much energy does it take (on average) to produce 1 kilogram of the following materials?". Low-Tech Magazine. 2014-12-26. Retrieved 2017-04-18.
- Halden RU (2010). "Plastics and health risks". Annual Review of Public Health. 31: 179–94. doi:10.1146/annurev.publhealth.012809.103714. PMID 20070188.
- Narayanan S (12 December 2005). "The Zadgaonkars turn carry-bags into petrol!". The Hindu. Archived from the original on 2012-11-09. Retrieved 1 July 2011.
- Substantial parts of this text originated from An Introduction to Plastics v1.0 by Greg Goebel (1 March 2001), which is in the public domain.
|Wikimedia Commons has media related to Plastics.|
|Wikiquote has quotations related to: Plastic|
- "J. Harry Dubois Collection on the History of Plastics, ca. 1900–1975". Archives Center, National Museum of American History, Smithsonian Institution. Archived from the original on 2006-02-12.
- "Material Properties of Plastics – Mechanical, Thermal & Electrical Properties". Plastics International. Archived from the original on 2017-03-24.
- "Plastics Historical Society".
- "History of plastics, Society of the Plastics Industry". plasticsindustry.org. Archived from the original on 2009-07-06.
- Knight L (17 May 2014). "A brief history of plastics, natural and synthetic". BBC Magazine.
- "Timeline of important milestone of plastic injection moulding and plastics". Tangram Technology Ltd. 27 June 2014.